DEFENSE TECHNICAL INFORMATION CENTER
DTICfhas determined on *I /$&-£&/J that this Technical Document has the Distribution Statement checked below. The current distribution for this document can be found in the DTICf Technical Report Database.
2) DISTRIBUTION STATEMENT A. Approved for public release; distribution is unlimited.9|j^\fc>H © COPYRIGHTED. U.S. Government or Federal Rights License. All other rights and uses except those permitted by copyright law are reserved by the copyright owner. I | DISTRIBUTION STATEMENT B. Distribution authorized to U.S. Government agencies only (fill in reason) (date of determination). Other requests for this document shall be referred to (insert controlling DoD office). ] DISTRIBUTION STATEMENT C. Distribution authorized to U.S. Government Agencies and their contractors (fill in reason) (date determination). Other requests for this document shall be referred to (insert controlling DoD office). ] DISTRIBUTION STATEMENT D. Distribution authorized to the Department of Defense and U.S. DoD contractors only (fill in reason) (date of determination). Other requests shall be referred to (insert controlling DoD office). ] DISTRIBUTION STATEMENT E. Distribution authorized to DoD Components only (fill in reason) (date of determination). Other requests shall be referred to (insert controlling DoD office). ] DISTRIBUTION STATEMENT F. Further dissemination only as directed by (insert controlling DoD office) (date of determination) or higher DoD authority. Distribution Statement F is also used when a document does not contain a distribution statement and no distribution statement can be determined. ] DISTRIBUTION STATEMENT X. Distribution authorized to U.S. Government Agencies and private individuals or enterprises eligible to obtain export-controlled technical data in accordance with DoDD 5230.25; (date of determination). DoD Controlling Office is (insert controlling DoD office).
Final Report for Phase I AFOSR STTR Project MULTIFUNCTIONAL NANOCOMPOSITE STRUCTURES VIA LAYER-BY-LAYER ASSEMBLY PROCESS February 14,2011 Sponsored by Air Force Office of Scientific Research Proposal # F09B-T36-0241, topic AF09-BT36
Name of Contractor:
Nico Technologies Corp. and University of Michigan
Dr. Kelechi C. Anyaogu ([email protected]
Dr. Nicholas A. Kotov ([email protected]
401 W. Morgan Road 48108, Ann Arbor, MI, USA
Title of Work:
Multifunctional Nanocomposite Structures via Layer-by-Layer Assembly Process
EXECUTIVE SUMMARY Current report is generated under Phase I STTR award on topic AF09-BT36. The overall goal of this project is to achieve large scale high-throughput manufacturing of multifunctional nanocomposites, which are comparable in physical characteristics to the standard aerospace composites, based on layer-by-layer (LBL) assembly process. To achieve this main objective, we proposed to: (1) construct and manufacture a new and fast LBL deposition machine (2) Realize exponential growth of LBL films with polyurethanes (PUs); (3) evaluate mechanical properties of the produced films; (4) manufacture large scale laminates of the free-standing films by consolidation. Using the new LBL deposition machine, dubbed 'Turbo LBL'. the depositon process was accelerated by ca. 100 times compared to traditional LBL deposition systems. The Turbo LBL system is compatible with a variety of nanomaterials and polyelectrolyte solutions which are typically used in traditional LBL assembly process. We demonstrated production of 10" x 40" size free standing LBL sheets at unprecedented rates, unattainable by conventional dip-dry LBL methods. Large size laminates of the free-standing LBL sheets made from graphene oxide (GO) and polyurethane (PU) polymers were fabricated. Mechanical property testing of the laminate samples indicated high extensibilities reaching 200%, and an overall excellent toughness. These promising results lay foundation for further optimization and their scale up manufacturing in Phase II. RESULTS OBTAINED IN THE PROJECT Task 1: Construction and manufacturing of a new LBL machine "Turbo LBL ". As described in the original proposal, the typical devices used in the deposition of LBL components sequentially transfer glass slides or other substrates from solution to solution. This system ultimately consists of adsorption of one component (eg. polymer), rinsing, drying, adsorption of another LBL component (eg. nanotubes), and another rinsing and drying steps. This approach of fabrication of LBL coatings and free-standing films require substantial amount of time. As a result, our task was to eliminate this problem by designing and constructing a continuous LBL deposition machine that will not only significantly accelerate the rate of deposition, but also produce films with comparable physical characteristics as observed from the conventional methods. The initial design schematics is depicted in Figure 1. On this fundamental idea, Turbo LBL machine was designed and developed applying an entirely new technology of LBL systems using proprietary know-how of Nico Technologies personnel. 2
During the project time period preceding this report, we designed and constructed two Turbo LBL machines, which are identified as Turbo LBL I and Turbo LBL 2. They are similar in concept but different in capacity and operations of the nozzles. Turbo LBL 2 is more advanced and most of the results will be referred to this latest design of the hardware. The heart of both Turbo LBL deposition systems is a rotating cylindrical substrate, or a drum (Figure 1). The latter rotates around the vertical axis while the aqueous dispersions/solutions are sprayed from the stationary nozzles positioned in four quadrants around the drum. The quadrants are separated by the spray shields and air-knives to avoid
the transfer of the mist from adjacent quadrants. As the drum rotates a vertical
section of its surface is sprayed by polymer solution, solution,
repeating the characteristic sequence of the LBL deposition but without timeconsuming transfer of the substrate from one beaker to another. Turbo LBL has some similarities with existing sprayLBL systems but they utilize alternate
Figure 1. Original schematics of Turbo LBL I (top view).
spraying. For instance, a flat surface is sprayed first with a solution of a polymer for a certain period of time, and then the same surface is sprayed with water for some period of time, nanoparticles, and water again. Alternate spray systems result in faster deposition rates than traditional LBL, but they are still relatively time consuming and often give poor uniformity of the coatings. Our system utilizes continuous spray without interruptions, which makes possible acceleration of the deposition in respect to the alternate spray systems by, at least 8 times. The multiple nozzles distributed along the vertical axis of the cylindrical substrate in Turbo LBL and air knives between the quadrants provide highly uniform multilayers. Our hardware solutions eliminate complicated robotic devices and provide continuous deposition of LBL composites. Additionally, Turbo LBL system has only one moving part, and for that reason, is exceptionally reliable and easy to maintain.
Task 1-1. Testing of performance of Turbo LBL Typically, the substrate of choice is held firmly onto the central drum and held in place with a hose-clamp. We tested various substrates such as Teflon, polycarbonate, and fabrics (Figures 2 and 3). The solution and water pumps are easily regulated to desired flow rates. Steady compressed air flow provided through the air blades facilitates drying after rinsing with water. Free-standing LBL films can be easily produced from LBL colloidal and polyelectrolyte solutions typically used in the conventional dipping LBL method when assembled on Teflon substrate (Figures 2). The surface of the substrate can be pre-treated by deposition of thin film of cellulose acetate to enhance adsorption of the initial LBL components. After deposition, the LBL film can be detached easily with slight application of acetone (for polycarbonates) or without (as with Teflon).
Figure 2 Photographic images of (A) LBL coating of PDDAPAA on Teflon substrate on TurboLBL2. (B) PDDA- PAA LBL coating (TOO bilayers) on Teflon. (C) Detachment of LBL film. (D) The free standing PDDA-PAA LBI. film.
Figure 3. (A) LBL coating of Kevlar fabric using. (B) Claypolymer coated Kevlar fabrics. (C) 10" x 40" LBL sheet made on Turbo LBL machine. (D) SEM image of surface of the coated Kevlar fabric
Task 2. Realization of exponentially erowine LBL films and preparation of laree size LBL sheets. Free standing LBL sheets were made from polyurethane (PU) and polyacrylic acid (PAA) solutions (lwt.%), both of which are known exponential LBL polyelectrolytes. A method of incorporating nanomaterials [eg. clay nanosheets, silica (Si02) nanoparticles, and graphene oxide (GO) nanosheets] to the LBL films was realized by mixing the PAA solution with the nanocolloids yielding a homogenous solution mixture. The large-size free-standing LBL sheets were build-up on polycarbonate substrate (Figure 4B). To facilitate better adhesion of the LBL
films, the substrate was coated with two bilayers of poly(diallyl dimethylammonium) chloride [PDDA] and PAA. This approach also enables easy detachment of the LBL sheets (Figure 4B). The substrate is then simply washed with water and can be re-used for further LBL film
combination of exponential LBL, spraying and highspeed rotation mechanism of Turbo LBL makes for the fast LBL film fabrication. We obtained several LBL
Figure 4. Photographs of (A) Turbo LBL2; (B) detachment of PU/PAA(clay)30 LBL sheet; (C) the 9"x 40" free-standing LBL sheet; (D) demonstration of robustness and flexibility of the LBL sheet - wrapping around a 4 inch diameter.
coatings and free-standing films with thicknesses reaching 450 um in ca. 30 minutes at speed of 2RPM. It would have taken more than from 10 to 500 hours to reach similar thickness of LBL films with the conventional dip-dry devices at their optimal deposition speeds depending on the deposition system used. GO was synthesized following modified Hummer's method1
nanosheets can be assembled in LBL structures
exponential LBL polyelectrolytes (Figure 5B). The GO LBL nanocomposites reveal some fascinating properties as seen in the
Figure 5. (A) AFM image of GO nanosheets. (B) Cross-section SEM image of GO/PVA nanocomposites (6:1); (C) CTE plots at different GO/PVA ratios.
thermal expansion plots (Figure 5C). At given ratios, the coefficient of thermal expansion (CTE) of the GO/PVA nanocomposite, for example, remains virtually unchanged. Such a unique property can be very valuable in several structural aerospace applications. Task 3: Evaluation of mechanical properties ofGO/PU films. The mechanical testing of the GO composite sheets (Fig. 3C) and laminates (Fig. 7) were carried out using Instron Q Systems model 100 (Test Resources) on small sample strips of width < 1.5 mm. Figure 6 and table 1 show mechanical testing data of the GO composites and comparison
structural materials. The toughness (K) of the GO composite was calculated to be ~ 52 MJ/m3 with elongation at break of 200%. The toughness recorded here is more than 27 times higher than previously reported value for toughness
of GO-polyelectrolyte LBL multilayers (1.9 MJ/m ) and with elongation at only 20%.2 It is also more than 70 times higher
Figure 6. (A) Representative stress-strain curve for the GO composite.
than the values reported for LBL nanocomposites reinforced with metal nanowires and nanoparticles3'4, as well as silk-clay composites.5 Materials GOPU composite (Nico Tech & UM) Aluminum alloy 1199-0 Airex® C70 Structural Foam Balsa Wood Core (Baltek® SB) Polycarbonate sheet (McMaster-Carr) Nylon
Elongation at break (%) 200
Specific gravity (e/cm3) 1.5
60-70 GPa 230 MPa
Tensile strength (MPa) 42
Table 1. Comparison of mechanical properties with some conventional materials.
Current GO composites possess impressive toughness and strain far exceeding any graphene oxide composite reported so far. The relatively low tensile strength value is attributable to the inherent structural nature of the individual composite sheets which reveal a porous internal network (Figure 7B inset). The ductile nature of the GO composite can be due to the PU backbone.6 Incorporation of cross-linking inorganic or organic moieties in the GO composite matrix can potentially enhance the tensile strength.7
Figure 7. Photographic images of (A) GO LBL composite laminate coupons. Each coupon comprises of 5 LBL sheets Inset shows the lamination process using Carver Hydraulic Unit 3912. The sheets are sandwiched between two Teflon slabs and hot-pressed for 40 minutes. (B) Demonstration of flexibility of the laminate coupons. Inset shows the cross-section SEM image.
Task 4: Preparation of large scale laminates by consolidation. Consolidation was achieved via hotpressing of individual free-standing LBL sheets made by Turbo LBL 2 (Figure 7A inset). No adhesive was needed
lamination of the prepared composites
Figure 8. Photographic images of representative GO composite laminate coupon (4" x 6" x 2 mm).
due to the elasticity of the material imparted by poly(urethane), PU, utilized as one of the LBL partners for GO nanosheets. With Turbo LBL deposition system and consolidation technology demonstrated, LBL composites definitely transcend the realm of microscale devices into the realm of high performance macroscale components. This achieved objective demonstrated that GO composite materials with impressive mechanical properties can be made in both large sizes and thicknesses (Figure 8), thereby paving the way for their further optimization and development. CONCLUSIONS AND RECOMMENDATIONS FOR PHASE I In the time period since commencement of this Phase I project, we have accomplished the following milestones/objectives:
Milestone 1: Designed and constructed a continuous LBL deposition system. A robust and versatile LBL deposition system that allows application of up to four different LBL solution or polyelectrolyte components was designed and manufactured. The new LBL system demonstrates a fast, high-throughput, environmentally benign, and low-cost manufacturing technique for LBL composite sheets with tailored properties. Milestone 2: Demonstrated production of large size LBL sheets exceeding all reported LBL multilayers made by conventional techniques We achieved LBL deposition on a variety of substrates including fabrics, polycarbonate and Teflon. The detached LBL sheets measured up to 10" x 40", which is greater than all reported
free-standing films made from polymers or
composite materials by any of the conventional techniques. The dimensions of the LBL materials made now are sufficiently large to manufacture many parts of unmanned aerial vehicles (UAVs) or some fairly small but critical parts of conventional planes Milestone 3: Realized highest toughness value for GO composite reported so far. The impressive results obtained in Phase I lay the pathway for optimization of structure and deposition conditions that will yield substantially better results in Phase II. Milestone 4: Realized consolidation of LBL sheets in large sizes.
References 1. Marcano, D.C. et. al., ACSNano, 2010, 4 (8), 4806-^814. 2. Kulkarni, D.D.; Choi, I.; Singamaneni, S.S.; Tsukruk, V.V. Graphene Oxide-Polyelectrolyte Nanomembranes. ACS Nano, 2010, 4 (8), pp 4667^676. 3. Ko, H.; Jiang, C; Tsukruk, V. V. Encapsulating Nanoparticle Arrays into Layer-by-Layer Multilayers by Capillary Transfer Lithography. Chem. Mater. 2005, 17, 5489-5497. 4. Gunawidjaja, R.; Jiang, C; Pelshanko, S.; Ornatska, M.; Singamaneni, S.; Tsukruk, V. V. Flexible and Robust 2D Arrays of Silver Nanowires Encapsulated within Free-standing Layerby-Layer Films. Adv. Fund Mater.2006,16, 2024-2034. 5. Kharlampieva, E.; Kozlovskaya, V.; Gunawidjaja, R.; Shevchenko, V.; Vaia, R.; Naik, R.; Kaplan, D.; Tsukruk, V. V. Flexible Silk-Inorganic Nanocomposites: From Transparent to Highly Reflective. Adv. Fund. Mater. 2010, 20, 840-846. 6. Kim, H.; Abdala, A.; Macosko, C. Graphene/Polymer Nanocomposites. Macromolecules, S
2010,43,6515-6530. 7. Podsiadlo, P.; Kaushik, A. K.; Arruda, E. M.; Waas, A. M; Shim, B. S.; Xu, J.; Nandivada, H.; Pumplin, B. G.; Lahann, J.; Ramamoorthy, A.; Kotov, N. A. Ultrastrong and Stiff Layered Polymer Nanocomposites. Science 2007, 318, 80-83.
*•** 3233 Andora Dr.. YDSilanti Ml 48198 USA
Manufacturing: 401 W Morgan Rd. Ann Arbor Ml 48108 USA
Dear Officer, Please find enclosed two copies of the Final Technical Report on the Phase I STTR AFOSR Project titled "Multifunctional nanocomposite structures via layer-by-layer assembly process", contract # FA9550-10-C-0129.
Elvira Stesikova, PhD, MBA Project Manager Nico Technologies Corp.